Phase Transformation and Deformation Model for Phase Transformation and Deformation Model for...
Embed Size (px)
Transcript of Phase Transformation and Deformation Model for Phase Transformation and Deformation Model for...
Phase Transformation and Deformation Model for Quenching Simulations Y. Kaymak VDEh Betriebsforschungsinstitute GmbH, Düsseldorf, NW, Germany Introduction In materials science, quenching is the rapid cooling of a workpiece to obtain certain material properties. For instance, quenching can reduce the crystal grain size of metallic materials and increasing their hardness. The rapid cooling prevents undesired phase transformations from occurring by reducing the window of time during which these undesired phase transformation are thermodynamically and kinetically favorable. The process of steel quenching is a progression, beginning with heating the sample up to a precise temperature, which is between 815°C and 900°C for the most of the steel types. The temperatures throughout the workpiece should be kept as uniform as possible during the heating. Afterwards, the workpiece is rapidly cooled usually by soaking in a fluid bath. Similar to the heating step, it is important that the temperature throughout the sample remains as uniform as possible during soaking. Often, the workpiece is excessively hard and brittle after quenching. In some cases, one or more tempering process steps are performed additionally in order to increase the toughness. In a tempering sub-process, the quenched steel is heated up to some critical temperature for a certain period of time, and then allowed to cool. The typical temperature evolution during the heat treatment process is show in Figure 1.
Figure 1. Temperature evolution during a typical heat treatment process. Heat treatment of the advanced steel grades (like micro-alloyed steels or AHSS steel grades) is a challenging process as the residual stress/deformation are pronounced and the quality requirements of the customers are getting tighter. A comprehensive modelling of the complex phenomena to estimate the
residual stress and deformation is essential for developing an optimal process control. The basis of the complex quenching model presented in this paper is developed within author’s PhD thesis . The model consists of a series of coupled physics, which are summarized in Figure 2. These coupled fields are solved by using the physics interfaces in COMSOL Multiphysics®. The temperature field is solved by the heat transfer in solids physics. The micro- structure field is modelled using kinetic expressions and domain ODEs and DAE physics. The displacement field is solved using the solid mechanics physics including the volume change (due to the temperature and micro-structure changes), plasticity, transformation induced plasticity (trip), creep, and large deformations. The constitutive model parameters as well as the isothermal and martensitic transformation kinetic parameters are validated and calibrated by several dilatometry tests.
Figure 2. Coupling of fields in quenching process. Theory and Governing Equations The quenching simulation model is focused on the cooling since the most significant part of the residual stress and deformation is developed during this rapid cooling. The model presented here consists of strongly coupled phenomena of heat transfer, micro- structure change, deformation (due to the thermal shrinkage, microstructure change related dilatation, trip, creep, plasticity, and large deformations). The governing fields involved in the quenching process and their interactions are shown in Figure 2. In quenching, the temperature field is controlled by the cooling boundary conditions. The temperature
Excerpt from the Proceedings of the 2017 COMSOL Conference in Rotterdam
evolution drives the phase transformation kinetics and phase transformations are accompanied by latent heat release. Moreover, all the material properties depend on the temperature and microstructure. A linear mixture rule is used for the Young’s modulus 𝐸𝐸, Poisson’s ratio 𝜈𝜈, initial yield stress 𝜎𝜎𝑦𝑦0, heat capacity 𝐶𝐶𝑝𝑝 and thermal conductivity 𝑘𝑘. However, a harmonic mixture rule is used for the density 𝜌𝜌. 𝐸𝐸 = 𝑓𝑓𝑎𝑎𝐸𝐸𝑎𝑎(𝑇𝑇) + 𝑓𝑓𝑏𝑏𝐸𝐸𝑏𝑏(𝑇𝑇) + 𝑓𝑓𝑚𝑚𝐸𝐸𝑚𝑚(𝑇𝑇) 𝜈𝜈 = 𝑓𝑓𝑎𝑎𝜈𝜈𝑎𝑎(𝑇𝑇) + 𝑓𝑓𝑏𝑏𝜈𝜈𝑏𝑏(𝑇𝑇) + 𝑓𝑓𝑚𝑚𝜈𝜈𝑚𝑚(𝑇𝑇) 𝜎𝜎𝑦𝑦0 = 𝑓𝑓𝑎𝑎𝜎𝜎𝑎𝑎𝑦𝑦0(𝑇𝑇) + 𝑓𝑓𝑏𝑏𝜎𝜎𝑏𝑏𝑦𝑦0(𝑇𝑇) + 𝑓𝑓𝑚𝑚𝜎𝜎𝑚𝑚𝑦𝑦0(𝑇𝑇) 𝐶𝐶𝑝𝑝 = 𝑓𝑓𝑎𝑎𝐶𝐶𝑝𝑝𝑎𝑎(𝑇𝑇) + 𝑓𝑓𝑏𝑏𝐶𝐶𝑝𝑝𝑏𝑏(𝑇𝑇) + 𝑓𝑓𝑚𝑚𝐶𝐶𝑝𝑝𝑚𝑚(𝑇𝑇) 𝑘𝑘 = 𝑓𝑓𝑎𝑎𝑘𝑘𝑎𝑎(𝑇𝑇) + 𝑓𝑓𝑏𝑏𝑘𝑘𝑏𝑏(𝑇𝑇) + 𝑓𝑓𝑚𝑚𝑘𝑘𝑚𝑚(𝑇𝑇)
𝜌𝜌 = 1
+ 𝑓𝑓𝑏𝑏𝜌𝜌𝑏𝑏(𝑇𝑇) + 𝑓𝑓𝑚𝑚
where the subscripts 𝑎𝑎, 𝑏𝑏 and 𝑚𝑚 correspond to the austenite, bainite and martensite microstructure volume fractions. 𝑇𝑇 stands for the temperature and 𝑓𝑓 represents the volume fraction of the microstructure. For the sake of simplicity a perfectly plastic behavior can be assumed if needed. The heat generation due to dissipation of mechanical energy has no significant influence on the temperature field. Similarly, the stress dependency of the transformations can also be discarded. So, these two coupling phenomena greyed-out in Figure 2. The temperature field is solved by the heat transfer in solids physics in COMSOL Multiphysics® software. The micro-structure field is modelled at integration point level using kinetic expressions and domain ODEs and DAE physics. The displacement field is solved using the solid mechanics physics including the volume change due to the temperature and micro- structure changes. This volumetric strain is given by:
𝑑𝑑𝑑𝑑 = �𝜌𝜌𝑎𝑎(𝑇𝑇ref)𝜌𝜌 3 − 1
where 𝑇𝑇ref is the strain reference temperature 𝜌𝜌𝑎𝑎 is the austenite density and 𝜌𝜌 is the mixture density. It is assumed that initial microstructure is completely austenite. Moreover, the nonlinear phenomena like plasticity, transformation induced plasticity (trip), creep, and large deformations are also considered in the solid mechanics physics setup in COMSOL. The governing partial differential equations (PDEs) and expressions of the model are further discussed on the following sub-sections.
Temperature field: The temperature field in solid material is modelled by the heat transfer in solids physics:
𝜌𝜌𝐶𝐶𝑝𝑝 𝜕𝜕𝑇𝑇 𝜕𝜕𝜕𝜕
+ ∇ ∙ 𝐪𝐪 = 𝑄𝑄
𝐪𝐪 = −𝑘𝑘∇𝑇𝑇
where, ρ is the density, 𝐶𝐶𝑝𝑝 is the heat capacity, 𝑇𝑇 is temperature field, 𝜕𝜕 is the time, 𝐪𝐪 is heat flux vector, 𝑘𝑘 is the heat conductivity, 𝑄𝑄 heat source due to the latent heat of the phase transformations. The equation for the heat source 𝑄𝑄 depends on the transformation latent heats as well as the phase transformation rates. It is defined by: 𝑄𝑄 = 𝑑𝑑𝑎𝑎𝑏𝑏𝑓𝑓�̇�𝑏 + 𝑑𝑑𝑎𝑎𝑚𝑚𝑓𝑓�̇�𝑚
where, 𝑑𝑑𝑎𝑎𝑏𝑏 and 𝑑𝑑𝑎𝑎𝑚𝑚 are the latent heats of the austenite to bainite and austenite to martensite transformations, 𝑓𝑓�̇�𝑏 and 𝑓𝑓�̇�𝑚 are the rates of the austenite to bainite and austenite to martensite transformations, respectively. For the sake of simplicity, the temperature field in the quenching medium is not modelled. Instead, either the temperature or heat flux at the solid boundaries are defined, e.g., by using convective heat transfer coefficients and radiation to ambient. Microstructure field: There are two types of transformations relevant to this study: (1) austenite to bainite transformation, which is diffusion controlled, needs an incubation time before the transformation starts. (2) Austenite to martensite transformation, which is diffusionless, is controlled only by temperature that means it can be expressed as a function of temperature without solving or integration a PDE. The austenite to bainite transformation is modelled using the domain ODEs. The transformation kinetics for the bainite formation is assumed to obey the Scheil’s addition rule and Johnson-Mehl-Avrami- Kolmogorow (JMAK) equation. Two state variables per integration point are defined, one for the Scheil’s sum and the other for bainite volume fraction in JMAK-equation. The Scheil’s sum 𝑠𝑠𝑠𝑠 is obtained by integrating:
𝑠𝑠�̇�𝑠 = 1
The incubation time is completed when the Scheil’s sum reaches the unity. After this incubation time, the
Excerpt from the Proceedings of the 2017 COMSOL Conference in Rotterdam
bainite volume fraction 𝑓𝑓𝑏𝑏 is obtained by integrating JMAK-equation: 𝑓𝑓�̇�𝑏 = 𝐾𝐾 ∙ 𝑛𝑛 ∙ 𝜕𝜕𝑛𝑛−1 ∙ exp(−𝐾𝐾 ∙ 𝜕𝜕𝑛𝑛)
where, 𝑛𝑛 is known as JMAK-exponent and 𝐾𝐾 is JMAK-factor. They are calculated using the bainite transformation start time 𝐵𝐵𝑠𝑠(𝑇𝑇) and finish time 𝐵𝐵𝑓𝑓(𝑇𝑇). These start and finish curves are given in the Time-Temperature-Transformation (TTT) diagrams. If it is assumed that the bainite volume fraction 𝑓𝑓𝑏𝑏 is 0.01 at the starti